obtaining Hydrostatic or Pressure Design Basis for " Fi berg liss'; (G lassfi berrei nforced Thermosetti n gresi n) Pipe and Fittingsl


 Margaret Reed
 11 months ago
 Views:
Transcription
1 t,.altt\. 4Ll lttt Designation: D (llt. 4/l g r_ NTERNAf'ONAL aa L. Scope* Standard Practice for obtaining Hydrostatic or Pressure Design Basis for " Fi berg liss'; (G lassfi berrei nforced Thermosetti n gresi n) Pipe and Fittingsl An American National Slai! This standard is issued under the fixecl designation D 2992; the number immediately following the designation indicates the year of original adoption or. in the case of revision, the year of last revision. A number in parentheses indicates the year of last reappror el A superscript epsilon (e) indicates an editorial change since the last revision or leappro\3. This stanrlard has been approved Jrtr use by agencies of the Depurtment of Deknse'. This practice establishes two procedures, Procedure A (cyclic) and Procedure B (static), for obtaining a hydrostatic design basis (HDB) or a pressure design basis (PDB) for fiberglass piping products, by evaluating strengthregression data derived from testing pipe or fittings, or both, of the same materials and construction, either separately or in assemblies' Both glassfiberreinforced thermosettingresin pipe (RTRP) and glassfiberreinforced polymer mortar pipe (RPMP) are fiberglass pipe. Nore lfor the purposes of this standard, polymer does not include natural polymers..2 This practice can be used for the HDB detemination for fiberglass pipe where the ratio of outside diameter to wall thickness is l0: or more. Nore 2This limitation, based on thinwall pipe design theory, serves further to limit the application of this practice to internal pressures which, by the hoopstress equation, are approximately 20 % of the derived hydrostatic design shess (HDS). For example, if HDS is 5000 psi ( kpa), the pipe is limited to about 000psig (6900kPa) internal pressure, regardless of diameter..3 This practice provides a PDB fbr complexshaped products or systems where complex stress fields seriously inhibit the use of hoop stress..4 Specimen end closures in the underlying test methods may be either restrained or free, leading to certain limitations'.4. Restrained Endsspecimens are stressed by internal pressure only in the hoop direction, and the HDB is applicable for stresses developed only in the hoop direction..4.2 Free Endsspecimens are stressed by internal pressure in both hoop and longitudinal directions, such that the This practice is under the jurisdiction of ASTM Committee D20 on Plastics and is the direct responsibility of Subcommittee D20.23 on Reinforced Plastic Piping Systems and Chemical EquiPment. Cunent edition approved Oct. 5, Published November 2006 Originally approved in 97. Last previous edition approved in 200 as D2992Ol' hoop stress is twice as large as the longitudinal stress. l practice may not be applicable for evaluating stresses indut by loadings where the longitudinal stress exceeds 50 % oltl HDS..5 The values stated in inchpound units are to be regardi as the standard. The values in parentheses are given information purposes only. NorE 3There is no similar or equivalent SO standard..6 This standard does not purport to address all ojrt safery concerns, if any, associated with its use' t ist responsibility of the user of this standard to establish appr' priate sat'bty and health practices and determine the applr bilitl, of regulatory limitations prior to use. 2. Referenced Documents 2. ASTM Srundards: 2 D 68 Practice for Conditioning Plastics for Testing f 883 Terminology Relating to Plastics i) 598 Test Method for TimetoFailure of Plastic lr Under Constant nternal Pressure ] 599 Test Method for Resistance to ShortTime Hydn lic Pressure of Plastic Pipe, Tubing, and Fittings D 6(Xi Terminology for Abbreviated Terms Relating Plastics D 243 Test Method for Cyclic Pressure Strength of RrL forced, Thermosetting Plastic Pipe D 3567 Practice for Determining Dimensions of "Flh glass" (GlassFiberReinforced Thermosetting Resin) li and Fittings F4lf Terminology Relating to Plastic Piping Systems F 948 Test Method for TimetoFailure of Plastic Prpi Systems and Components Under Constant nternal Prt sure With Flow 2 For ref'erenced ASTM standards, visit the ASTM website, wwwastmo[ contact ASTM Customer Seruice at Annual BookoiA! Starulards volume information, refer to the standard's Document Summarypul the ASTM website. 2.2 SO Stant 3 Preferred 3. Terminology 3. Definitiont 3.. Generalnologies D 883 a. with Terminolog, 3..2 closure, fastened to the en produces longitur radial stresses in 3..3 closure, nism which relie external structur pressure, thereby the hoop and rad 3..4 failurebody of the sper fracture, localize than one diamete Nore 4For this included as failures fiberglas fiber reinforcemr thermosettingres gregate, granular ments, or dyes; t ings may be inclr 3..6 reinforce pipe with aggreg 3..7 reinforce glass pipe withor" 3..8 hoop strt product in the ci sure; hoop stress follows: where: S = hoop stres D = average re P = internal pl tr = minimum Nore 5Hoop st cylindrical specimen based on pressure hydrosta, oped for fibergla service design far 3.l.lO hydrosn maximum interni *A Summary of Changes section appears at the end of this standard' ASTN/ nternational, 0O Barr Harbor Drive, PO Box C700, West Conshohocken, PA , United States 3r8 3 Available from An 4th Floor, New York,
2 ,([fpo2ee ls0 Standard: 3 Prefened Numbersseries of Preferred Numbers3 Terminology 3. Defnitions: 3,, GeneralDe{initions are in accordance with Termi D 883 and F 42, and abbreviations are in accordance Terminology D 600, unless otherwise indicated.,2 closure, freeenda sealins device or mechanism to the end of the test specimen so that interrral pressure longitudinal tensile stresses in addition to hoop and stresses in the test specimen. 3,.3 closure, restrainedenda sealing device or mechawhich relies on a rod through the test specimen or an $ructure to resist the end thrust produced by internal, thereby limiting the stresses in (straight) specimens to ehoop and radial directions only. 3,,4 failurethe transmission of the test fluid through the of the specimen in any manner, whether it be a wall,localized leaking, or weeping at a distance greater one diameter from the end closure Nom 4For this practice, specimens which have not failed may be as failures under the specific conditions given in 6.3, 9.3, and 3,.5 fiberglass pipea tubular product containing glass reinforcement embedded in or surrounded bv cured ngresin; the composite structure may contain aggranular or platelet fillers, thixotropic agents, pigor dyes; thermoplastic or thermosetting liners or coatmay be included. 3,,6 reinforced polymer mortar pipe (RPMP)a fiberglass with aggregate. 3,.7 reinforced thermosetting resin pipe (RTRP)a fiberpipe without aggregate. 3.L8 hoop sfressthe tensile stress in the wall of the piping in the circumferential direction due to internal preshoop stress will be calculated by the SO equation, as s: P(D t,)/2t, = hoop stress, psi (kpa), = over&ge reinforced outside diameteq in. (mm), = internal pressure, psig (kpa), and = minimum reinforced wall thickness. in. (mm). Nmr 5Hoop stress should only be determined on straight hollow ical specimens. Product evaluation of more complex shapes may be 0n Fessure. 3.,9 lrydrostatic design basis (HDB)a hoop stress develfor fiberglass pipe by this practice and multiplied by a design factor to obtain an HDS 3,0 hydrostatic design pressure (HDP)the, estimated imum internal hydrostatic pressure that can be applied ravailable from American National Standards nstitute (ANS), 25 W. 43rd St., floor, New York, NY 0036, () cyclically (Procedure A) or continuously (Procedure B) to a piping component with a high degree of certainty that failure of the component will not occur. 3.l.ll hydrostatic design stress (HDS)the estimated maximum tensile stress in the wall of the pipe in the hoop direction due to internal hydrostatic pressure that can be applied cyclically (Procedure A) or continuously (Procedure B) with a high degree of certainty that failure of the pipe will not occur longterm hydrostatic strength (LTHS) the estimated tensile stress in the wall of the pipe in the hoop direction due to intemal hydrostatic pressure that, when applied cyclically, will cause failure of the pipe after a specified number of cycles by Procedure A or a specified number of hours by Procedure B. Nors 6The time for determination of LHS or LTHP is soecified bv the product standard. Typically, the time is 50 X 06 or 657 x 06 cycles for Procedure A and or h for Procedure B longterm hydrostatic pressure (LTHP)the estimated interrral pressure of the piping product that, when applied cyclically, will cause failure of the product after a specified number of cycles by Procedure A or a specifled number of hours by Procedure B pressure design basis (PDB)an internal pressure developed for flberglass piping product by this practice and multiplied by a service design factor to obtain an HDP pressure rating (PR)the estimated maximum pressure in the pipe or fitting that can be exerted continuously with a high degree of certainty that failure of the piping component will not occur senice designfactora number equal to.00 or less that takes into consideration all the variables and degree of safety involved in a fiberglass piping installation so that when it is multiplied by the HDB, an HDS and corresponding pressure rating is obtained, or when it is multiplied by the PDB, a pressure rating is obtained directly, such that in either case a satisfactory and safe piping installation results when good quality components are used and the installation is made properly. 3.2 Definitions of Tenns Specifc to This Standard: 3.2. average outside diametera measurement obtained in accordance with Practice D 3567 less any veilreinforced and nonreinforced exterior coating thicknesses minimum reinforced wall thicknes.ra measurement obtained in accordance with Practice D 3567, excluding veilreinforced and nonreinforced coating and lining thicknesses; wall thickness of flttings is determined at the thinnest section of the fitting body. 4. Summary of Practice 4. Procedure A consists of exposing a minimum of 8 specimens of pipe or fittings, or both to cyclic internal pressures at a cycle rate of 25 cycles/min and at several different pressures. Elevated test temperatures are obtained by circulating a hot liquid through the specimens or by testing in an air environment where the temperature is controlled.
3 gily.ull D The cyclic LTHS or cyclic LTHP of a pipe or fitting is obtained by an extrapolation of a loglog plot of the linear regression line for hoop stress or internal pressure versus cycles to failure The experimental basis fbr Procedure A shall be in accordance with Test Method t]:43, which forms a part of this practice. When any part of the procedure is not in agreement with Test Method lf :43, the provisions of this practice shall be used Joints between pipe and fltting specimens shall be typical of those normally used for the kind of piping being 4.2 Procedure B consists of exposing a minimum of 8 specimens of pipe or fittings, or both, to constant internal hydrostatic pressures at differing pressure levels in a controlled to failure for HN: To characterize fiberglass piping products, it sary to establish the stress versus cycles or time to is nur failure,i pressure versus cycles or time to failure relationships three or more logarithmic decades of time (cycles or within controlled environmental parameters. Because of t nature of the test and specimens employed, no single liner adequately represent the data. Therefore, the confidencelimr should be established. 5.3 Pressure ratings for piping of various dimensions ater temperature may be calculated using the HDS determinedt orr hourr tested. environment and measuring the time 5.. An alternative design practice based on initial stn versus timetof'ailure relationships employs a strain basis instead of the stress basis HDB defined by rhis practice, i strain basis HDB is most often used for buried pipe desrgr with internal pressures ranging from 0 to 250 psig (.72MPr of piping provided that the same process and material are used both for test specimens piping in question. testing one size each pressure level. Test temperatures are obtained by immersing the specimens in a controlledtemperature water bath, by testing in an air environment where the temperature is con NorE 7Testing in tr water bath precludes the detection of weeping failure, (see 3."i) by either visual or electronic means. rl component. 5.5 Results obtained at one set of environmental verifiedr conditior should not be used for other conditions, except that hrgh temperature data can be used for design basis assignmenli lower application temperatures. The design basis shouldl for each specific piping product. Design tested. determined 4.3 The HDB category is obtained by categorizing the LTHS in accordance with Section or Section The PDB category is obtained by categorizing the LTHP in accordance with Section or Section l. 4.5 Hydrostatic design stresses for pipe are obtained by multiplying the HDB values by a service design factor. processing can significantly affect the longterm performmi of piping products, and therefore should be taken into consii eration during any evaluation. 5.6 This practice is valid for a given pipe or fitting only, long as the specimens are truly representative of that materi. and manufacturing process Changes in materials or manufacturing processesrri necessitate a reevaluation as described in Section Reconfirmation of HDB or PDB for Altered ConstrttctionsWhen a product already has an HDB or PDB determined in accordance with this practice and a change of process or material is made, a reconfirmation of the original HDB or PDB may be attempted in accordance with Section 2. At least six specimens must be tested and meet the specified Cyclic Hydrostatic Pressure 6. Select either freeend or restrainedend criteria. 5. Significance and al PROCEDURE A 6. LongTerm Cyclic Hydrostatic Strength or Use LongTen internal pressure versus timetofailure relationships, under selected internal and external environments which simulate actual anticipated product enduse conditions, tiom which a design basis for specific piping products and materials can be obtained. This practice defines an HDB for material in straight, hollow cylindrical shapes where hoop stress can be easily calculated, and a PDB for fittings and joints where stresses are each selected temperature D 243 except as follows: 6.2. in accordance with Test Determine the average outside diameter mum reinforced wall thickness D in bar Metlrr and the accordance with mn Pracl, Nore 9Because of the need to cut the specimen, this detenrunatr may be made on the failed test specimen. A corrected hoop stress isth more complex. 320 l0w the ambient air tem The s to obtain a di c c 00 0c 000r After 6.3 Anayz logarithm of logarithm of t llt Nore i or pressure on th axis A spe closure may b the 95 Vo lowe resumed provi a test joint, or Those cy the regression lower or highe lower confide satisfied. Norp l2*nor sion line recalcu Deten method of lea those nonfailu 6.3. and 6"3 pressures that average; deter cyclestofailur level, that is, a within closures on the tensile stresses induced by internal pressure and thetu of joint in the intended piping system (see l..t). 6.2 Obtain a minimum of 8 failure stresscycle pointsl 5. This practice is useful for establishing the hoop stress or Noro ing heat to Total tr Nors SScaling of fittings and joints should be further shorttime testing in accordance with Test Method D 599. air environmr tained within andtr rl 4.2. The static LTHS or stafic LTHP of a pipe or fitting is obtained by an extrapolation of a logog linear regression line for hoop stress or internal pressure versus time to failure The experimental basis fbr Procedure B shall be in accordance with either Test Method,) t5q8 or Test Method F 948, or both, which lbrm a part of this practice. When any part of this practice is not in agreement with the selected method, the provisions of this practice shall be used Joints between pipe and fitting specimens shall be typical of those normally used for the kind of piping being Elevt a heated test specrl 5.4 Pressure ratings at each temperature for componer other than straight hollow shapes may be calculated usingrl HDP determined by testing one size of piping provided thar, the specific materials and manufacturing process used foril test specimens are used for the components, (2) for joinfi joining materials and procedures used to prepare the specimens are used for field joining, and (J) scaling of crilrr dimensions is related to diameter and pressure rating of trolled, or by circulating a temperaturecontrolled fluid through the specimen. calculated for u '+20 pr points exclude identify them i Nors l3sinr recommended thz as one specimer together, with thr fails first, it can b pipe with a mech fail first, it can b, fitting fails. f thir obtain failure poir specimen.
4 ([Jp o2ee206 for use in the analysis. 6,2.2 Elevated test temperatures are obtained by circulating heated test liquid through the specimens or by testing in a hot environment. n either case the test liquid shall be mainwithin :5'F (3'C) of the selected temperature. Nom l0where elevated test temperatures are maintained by applyheat to the circulating test liquid, work to date indicates that the air temderature need not be controlled The stress or pressure values for test shall be selected obtain a distribution of failure points as follows: Cycles to Failure 000 to to to to After Total Failure Points at least 8 6,3 Lnalyze the test results by using, for each specimen, the of the stress or pressure in Section 6 and the of the cycles to failure, as described in Annex Ai. Noru lt is the custom of those testing flberglass pipe to plot stress pressure on the veftical (y) axis and time or cycles on the horizontal (r) 6.3. A specimen which leaks within one diameter of an end may be: () included as a failure point if it lies above Valower confidence limit curve; ( 2) repaired and testing provided the new leak is more than one diameter from test joint, or (3) discarded and no data point recorded. 6,3.2 Those specimens that have not failed after more than cycles may be included as failures in establishing rcgression line. Use of such data points may result in a or higher cyclic LTHS or cyclic LTHP. n either case, the confidence value requirements of Section 5 must be Nom l2nonfailed specimens may be left under test and the regresline recalculated as failures are obtained Determine the flnal line for extrapolation by the of least squares using the failure points along with nonfailure points selected by the method described in and Do not use failure Doints for stresses or that cause failure in less than 500 cycles on the determine these points by averaging the number of aiiure of tests made at the same stress or pressure that is, a stress within r200 psi (380 kpa) or a pressure 20 psig (38 kpa). nclude in the reporl all failure excluded from the calculation by this operation and them as being in this category. Nors l3since this procedure is for pipe or fittings, or both, it is that the pipe specimen and litting be tested at the same time one specimen, using the normal joining procedures to join them her, with the fitting being at one end of the specimen. f the fitting flnt, it can be cut off, and the test can be continued using the unfailed with a mechanical end closure replacing the fitting. Should the pipe first, it can be recorded and repaired and the test continued until the fails. f this recommendation is followed, it may enable the tester to falure points for both the pipe and the fitting while testing only one 7. Cyclic Hydrostatic Design Basis 7. Calculate the cyclic LTHS at the specified time (50X 06 or 657 x 06 cycles) as described in Annex A. 7.2 f Sxa > 0 (see Al.4) consider the data unsuitable. 7.3 Calculate r in accordance with A.4"3. f r is less than the applicable minimum value given in Table Al.l, consider the data unsuitable. 7.4 f required, determine the cyclic HDB category in accordance with Table. 8. Cyclic Pressure Design Basis 8. Use the procedures in 7.,.2, and 7.3, using pressure in place of stress. 8.2 f required, determine the cyclic PDB category in accordance with Table 2. PROCEDURE B 9. LongTerm Static Hydrostatic Strength 9. Select either freeend or restrainedend closures based on the tensile stresses induced by internal pressure and the type of joint in the intended piping system (see.4). 9.2 Obtain a minimum of 8 failure points for each selected temperature in accordance with Test Method D 598 or Test Method F 948 except as follows: 9.2. Determine the average outside diameter and the minimum reinforced wall thickness in accordance with Practice D 3567 (Note 9) The inside environment for the pipe or fitting, test specimens, or both, shall be water. The outside environment shall be air or a controlled temperature water bath (See 7). Other media may be used, but the environment shall be given in the test report. The test liquid shall be maintained within f 5'F (3'C) of the test temperature (Note 0) The stress or pressure values for test shall be selected to obtain a distribution of failure points as follows: rable Hydrostatic "::,F":$;"Categories by Procedure A Hydrostatic Design Basis Category psi^ s (kpa) Range of Calculated Values psl (kpa) (7 200) to 3 00 (6 500 to ) (2 700) to ( to ) ( to ( to ) (34 500) to (33 00 to ) (43 400) to (4 000 to ) (55 200) to ( to ) (68 900) to 990 ( to ) (86 200) to ( to ) (0 000) to ( to ) (38 000) to (3 000 to ) (72 000) to ( to ) (27 000) to ( to ) ( ) to ( to ) ^Standard stress levels chosen in accordance with SO 3, Series RO
5 TABLE 2 Pressure Design Basis Categories by Procedure A or Procedure B Pressure Design Basis Category Range of Calculated Values (ba " (kpa) psl (kpa) (6 3) (630) 87 to 0 (605 to 760) (8) (800) to 43 (765 to 990) (0) ( 000) 44to 72 (995 to 80) (2 5) ( 250).73 to 220 ( 90 to 50) (6) ( 600) 22 to 287 ( 520 to 980) (20) (2 000) 288 to 345 ( 990 to 2 380) (25) (2 500) 346 ro 438 (2 390 to 3 020) (3.5) (3 50) 439 to 556 (3 030 to 3 830) (40) (4 000) s57 to 695 (3 840 to 4 790) (50) (s 000) 696 ro 876 (4 800 to 6 040) (63) (6 300) 877 to 0 (6 050 to 7 680) (80) (8 000) s to 380 (7 690 to 580) (00) (0 000) 390 to 720 (9 590 to 800) (25) (2 500) 730 to 2220 ( 900 to 5 300) a Standard pressures chosen in accordance with SO 3, Series R.0. Hours to Failure 0 lo to After After Total Failure Points at leasl 3 at least at leasl Maintain the internal test pressure in each specimen witjrin + 7a of this pressure. Measure the time to failure to within +2 7o or 40 h, whichever is smaller. 9.3 Analyze the test results by using, for each failure point, the logarithm of the stress or pressure in poundforce per square inch or poundforce per square inch gage (kilopascals) and the logarithm of the timetof'ailure in hours as described in Annex,Al (Fiote!l) A specimen which leaks within one diameter of an end closure may be: () included as a failure point if it lies above the 95 Vo lower confidence limit curve; ( 2) repaired and testing resumed provided the new leak is more than one diameter from a test joint, or (3) discarded and no failure point recorded Those specimens that have not f'ailed after more than h may be included as failures in establishing the regression line. Use of such data points may result in a lower or higher static LHS or static LTHP. n either case, the lower confidence value requirements of must be satisfied. Nore l4 Nonfailed specimens may be left under test and the regression line recalculated as failures are obtained Determine the final line for extrapolation by the method of least squares using the failure points along with those nonfailure points selected by the method described in and!.3.2. Do not use failure points for stresses or pressures that cause failure in less than 0.3 h on the average; determine these points by averaging the timestofailure of tests made at the same stress or pressure level, that is, a stress within +200 psi (380 kpa) or a pressure within r20 psi (38 kpa). nclude in the report all failure points excluded from the calculation by this operation and identify them as being in this category (hi*te l2). 0. Static Hydrostatic Design Basis l0.l Calculate the static LTHS at the speci{ied time ( or h) as described in Annex Ai. 4$JP o 2ss2ol 0.2 f Sry > 0 (see Atr.4), consider the data unsuitable, 0.3 Calculate r in accordance with AX.4.3. f r is lesstii the applicable minimum value given in Tahlo,4., considr the data unsuitable. 0.4 f required, determine the static HDB categotl: accordance with T*hie l.. Static Pressure Design Basis. Use the procedures in li).tr, {}.2, and {}.3, usin pressure in place of stress..2 f required, determine the static PDB categoq r accordance with Tairle Reconfirmation of HDB or PDB 2. When a piping product has an existing HDB orpd, determined in accordance with Procedure A or Procedutel any change in material, manufacturing process, constructirtr or liner thickness will necessitate a screening evaluationl described in tr2.2, i2.3, :.4, 2"5, and Obtain failure points for at least two sets of specimel each set consisting of 3 or more specimens tested at the silr stress or pressure level, that is, a stress within +200 psi (3 kpa) or a pressure within +20 psi (38 kpa), as follows: 2.2. For Procedure A: Cycles to Failure (Average of Set) to lvlore than Total Failure Points at least 6 nclude as failures those specimens which have not latlt after cycles provided they exceed the existingh, or PDB regression line For Procedure B: Hours to Failure (Average of Set) 0 to 200 More than 000 Total Failure Points at least 6 nclude as failures those specimens which have not failr after 3000 h provided they exceed the existing HDB ot Pl regression line. 2.3 Calculate and plot the 95 7o confidence limits andtl 95 7o prediction limits of the original regression line accordance with Al..tr using only data obtained prior totl change. Nors 5Plediction limits define the bounds fbr single observatu whereas confidence limits define the bounds fbr the regression line, Nors 6 For 95 o/o confidence limits, there is a2.5 7o probabilitli the mean value for the regression line may fal above the UCL and a l.j probability that the mean value for the regression line may fall belor: LCL. For 95 o/o prediction limits, there is a 2.5 Vo probability t individual data points may tall above the UPL and a 2.5 % probabilrtit individual data points may faii below the LPL. 2.4 Consider any changes in the material or manufactur process minor and perrnissible if the results of l2.l meett followins criteria The level falls on original regrer The pressure level of the original The determined re individual fail line. 2.5 Altern material or mr 2.2 meet the 2.5. Alt c limit of the or At ' 3000h failure 72.6 Data t assumed to be line and HDB 2.7 f the c changes are cc be established. an interim HD be taken as thr 2.7.t The tained by ex c. failure points procedure in A 2..2 The regression line 3. Hydrostat Pressure 3. Obtain PDB as determ design factor s general groups manufacturing tions in the ma techniques, ant The second grc installation, en expectancy des Nore 7t is factors. The serr, engineer after eva properties of the Recommended se ASTM. 322
6 .([fp o 2ss The average failure point for each stress or pressure falls on or above the 95 7o lower confidence limit of the regression line. 2,4,2 The earliest individual failure point at each stress or level falls on or above the 95 7a lower prediction limit the original regression line The failure points are distributed about the originally ined regression line. No more than two thirds of the vidual failure points may fall below the original regression 2,5 Alternatively to tr2.4, consider any changes in the or manufacturing process permissible if the results of meet the following: U.5. All data points fall above the 95 7o lower confidence ofthe original regression line, and 2,5,2 N least two points exceed 4.5 x 0 o cycles or failure time. l2.6data meeting the criteria of 2.4 or 2.5 may be to be part of the original data set and a new regression and HDB or PDB determined using all failure points. 2.7 f the data fails to satisfy the criteria of 2.4 or 2.5. the are considered major and a new regression line must. While the new test program is being conducted, rnterim HDB or PDB for the material or process change may as the lower of the followrns: 27. The 95 Vo lowef confidence limit of the value obby extrapolating the failure points of 2.2. to 000 cycles (50 years) by the procedure in "2, or the points of to h (50 years) by the in Annex Al. 2,7.2 The 95 7o lower confidence of the original ion line at 50 years. lydrostatic Design Stress or Hydrostatic Design Pressure 3. Obtain the HDS or HDP by multiplying the HDB or as determined by Procedure A or Procedure B by a service factor selected for the application on the basis of two groups of conditions. The first group considers the ng and testing variables, specifically normal variain the material, manufacture, dimensions, good handling, and in the evaluation Drocedures in this method. second group considers the application or use, speciflcally environment, temperature, hazard involved, life desired, and the degree of reliability selected. 7t is not the intent of this practice to give service design The service design factor should be selected by the design after evaluating fully the service conditions and the engineering of the specific plastic pipe material under consideration service design factors will not be developed or issued by 4. Pressure Rating 4. For data based on hoop stress calculate the pressure rating from the HDS by means of the SO equation in 3..8 for each diameter and wall thickness of pipe made from the speciflc materials and constructions tested. 4.2 For data based on internal pressure, establish the pressure rating directly from the HDP for products made from the specific materials and constructions tested. 5. Report 5. Report the following information: 5.. Complete identification of the specimen including material type, source, manufacturer's name and code number, and previous significant history, if any Specimen dimensions including nominal size, average and minimum reinforced wall thickness, and average outside diameter, and liner material and liner thickness if product is lined Fitting dimensions, including all items listed in 5" N"2 and the type of fitting Procedure used, (Procedure A or Procedure B), and the ASTM designation of the underlying test method End closure type, freeend, or restrainedend Test temperature Test environment inside and outside of the pipe A table of stresses or pressures in poundforce per square inch or poundforce per square inch gage (kilopascals) and the number of cycles to failure (Procedure A) or timetofailure in hours (Procedure B) of all the specimens tested; the nature of the failures, and the part that failed, that is, fitting or pipe. Specimens that are included as failures after they have been under stress or pressure for more than cycles or more than l0 000 h shall be indicated The estimated LTHS or LHP The value for r. 5.l.l The HDB or HDP. l5.l.2 The source of the HDB or PDB (7. or.2 for Procedure A or l{}. or 0.2 for Procedure B), and the categorized value in accordance with Table or Table Any unusual behavior observed in the tests Dates of tests Name of laboratory and supervisor of tests. 6. Precision and Bias 6. The precision and bias ofthis practice for obtaining the HDB or PDB are as specified in Test Methods D t598, D 243, and [i 948. This practice includes a statistical basis for evaluating the suitability of the data in Sections 6 and Keywords 7. closure; cyclic pressure; design basis; flberglass pipe; reconfirmation: static Dressure 323
7 rflt\^ +lfrtlt.flhrrrynroor_06 e rj ANNEX (Mandatory nformation) A. LEAST SQUARES CALCULATONS FOR LONG.TERM HYDROSTATC STRENGTH OR LONGTERM HYDROSTAT PRESSURE Degrees of Freed (n2) ' A. General A.l.l The analysis is based on the following relationship: ydr0x (Ar.l) wnefe: ) = one variable, x = other variable, & = slope of the line, and a = intercept on the y axis. Al.l.2 A linear functional relationship analysis (sometimes called "covariance analysis") is used, subject to tests for the sign (that is, "+" or "") of the slope and the coefficient of correlation for the quantity of data available. The relevant equations are given together with example data and results, on the basis of which any other statistical computing package may be used subject to validation by agreement with the example results to within the indicated limits. A..3 For the purposes of this annex, a design service life of 50 years has been assumed. A.2 Procedure for Analysis of Data Al.2.l Use a linear functional relationship analysis to analyze n pairs of data values (as y and "x) to obtain the following information: A.2.. The slope of line, b, A.2..2 The intercept on the y axis, a, The correlation coefficient, r, and The predicted mean and the lower 95 7o confidence and prediction intervals on the mean value. A.3 Assignment of Variables A.3. Let x be log,ol, where / is the time, in hours (or cycles), and let y be loglo% where Vis the stress (or pressure) value. A.4 Functional Relationship Equations and Method of Calculation A.4. Basic Statistics and Symbols: Al.4.l. The following basic statistics and symbols are used: n = number of pairs of observed data values (Vi, t ), li = logro of V,, where Vr is the stress (or pressure) at failure of Observation i; i = l,... n, xi = log ro of /r, where r is the time to failure in hours of Observation i; i =,...n, ) = arithmetic mean of all y, values: n ' (A.2) x = arithmetic mean of all x,values: rat.  i2*, Relevant SumsofSquares: Calculate the following sumsofsquares anr crossproducts: S,,:;)(.r, ;)0r r) Al f Sry> 0, consider the data unsuitable for evalu ating the material; otherwise calculate also: s*:;)(r,x)2 s,,,: j>0,_ E, A.4.3 Correlation of Data: Calculate the coefficient of correlation, r, fromlh following relationship: r( t2.2 _ '"\) ' (.t.x,srr),:f7 't f the value of r is less than the applicah: minimum value given in Table A. as a function of n,reju the data; otherwise, proceed to A Functional Relationships: Al.4.4.l To find a and b for the functional relationship lirrr! = a + bx (Eq A.), first set: and then let: and then: ^: b: y5 (Ali fl),c \J,'/ TABLE A. Minimum Values for the Coefficient of Correlatior,', for Acceptable Data from n Pairs of Data (n2) 2 J 4 tc to r mtntmum (n2) r mrnrmum s o (Ali (Ajr ln o A L '0 2 3 tc Nore Al.ln Norn A.2Si the implied relatic A.4.5 Cah f t ' Ci statistics. For i fit, {, for true A'.2, Eq A. 324
8 ,([fp o2ee206 TABLE A.2 Student's "f " Value (TwoSided 0.05 Level of Significance) o grees of Freedom ln2) Student's" f'value t. 't Degrees of Freedom (n Student's "f'value, t" Degrees oj Freedom (n2) Student's "'Value, t" cl ) lu tl ' z. tj tc ol '20 ' s tjo ble an 'l ' t t 'l ' lht Non A rn generar,, ;;;.,:; r r. (A'ro) Nmr A.2Since.l'= log,,, Vand,r = log,o t, hence V= lo), /= l0'and Jreimplied relationship fbr V in terms of t is therefore: Y : 0(a+'x''8 ro ) A.4.5 Calculation of Vartances: Ai.4.5. f r.is the applicable time to failure, then set: x r: logrut, (,4.) A Calculate, in turn, the following sequence of statrstics. For i = to i = n, the best fit, {,, for true r, the best fiq [, for true ' and the error variance, ou, for x using Eq Al2, Eq A.3, and Eq '.4, respectively:,: {M, + (y,  a)b}/dt Y,: tt i bl, cr62: {)g'. ri)2+ )t)(r, 6,)':y{\(ll  2D A Calculate the following quantities: r  bourl2,!,,. D  2)tbo u2/n5,, B Dr(l +r) (Ar. r2) (A.3) (A.4) (A.s) (A.6) (Al.l7) A Calculate the following variances: the variance, C. of b usins the formula: C: D( + r) (A.8) 325
9 ,($fp o2ee2oo E  the variance, A, of a using the formula: ao{t'o*")*+} (A.9) the variance, o,,, of the fitted line at xrusing the formula: o,2 : A * 2Bxr* Cx.2 the error variance, o., for y using the fbrmula: o.2 : \oa 2 (A.20) (Al.2l) the total variance, or, fbr future values, yr_, for y at x.using the formula: or2  o,,2 + ou2 (A.22) A Calculate the estimated standard deviation, o' for y.using the equation: o,(o,,t +ou')ut (Ar.23) and the predicted value, y., for y at x.using the relationship:,7 a bxt (4t.24) where a and b have the values obtained in accordance with Eq Al.9 and Eq A Calcttlation and Confidence ntervals: Calculate the lower 957o prediction interval,!t o.ss, predicted for y.using the equation: )'ro.qs:)r.l,or (A.25) APPENDXES where: lr = value obtained in accordance with Eq A.24 whenr, is, as applicable, the value in accordance with q A. appropriate to a design life of, for example,5l years (that is, x (h)) or ro a time at whichji is desired to predict with 95 7o confidence the mrnj. mum value for the next observation of V, or = value obtained in accordance with Eq A.23, and tv = applicable value for Student's / for y = n  2 df,u given in Table A.2 for a twosided 0.05 level ol significance (that is, mean o). A Calculate the corresponding lower 95 Vo prediciv limit for V using the relationship: %0.e5 : oy'0" A The predicted mean value of V at time r,, thalji 7., is given by the relationship: VL:0t' where: YL = value obtained in accordance with Eq A.24. A Setting o, t= o,t in Eq A.22 will produce confidence interval for the line rather than a prediction intent for a future observation. (Ar (All X2.l Bas together with be used to va rounding errr ment, but acr of the results X2.2 Sum S* = 0.798( Syy = i S'y = o.o24t X2.3 Coe, r = Data Point 2 K o 7 8 X2.4 Funr ' 'll ' 2l 2( (Nonmandatory nformation) Xl. DATA ANALYSS , 4t 4( 5[ Xl. Hoop Stress versus CyclestoFailure or Timeto Failure: Xl.. Hoop stress is a more convenient parameter to use when attempting to predict longterm hydrostatic strength of a material. ts use reduces scatter in the data by compensating for varying dimensions in the test specimens. t effectively normalizes pressure for variations in specimen geometry, and reduces the variable to a material parameter. For this particular reason it has been widely used for evaluating the longterm hydrostatic properties of plastic materials. Essentially, once a value for HDS has been determined for a particular material and construction, that value can be used to effectively predict the longterm working pressure of tubular products by compensating for the various product geometries. Xl.l.2 The main limitation of the use of hoop stress is tlri it can only be applied to simple tubularshaped speciner Therefore, its application has been mainly limited to matenrl and a few products such as pipe and simple fittings lil couplings. Xl.2 ntetnal Pressure versus CyclestoFailure ortni tofailurethe use of internal pressure rather than sfti extends the application of this practice to the predictionr service life for many products of complex geometries whichl not permit the calculation of hoop stress. The logarithmt internal pressure is used in place of the logarithm of hoop stn in the calculations. J lo
10 ,([Jpo2ee206 xl Eq 50 rit ni AS of ion X2J Basic DataThe example data given in Table X2., together with the example analysis given in this appendix, can bused to validate statistical packages procedures. Because of munding enors, it is unlikely that there will be exact agreement, but acceptable procedures should agree within +0.' Vo of theresults given in X2.5. X2.2 Sums of Squares:," = J,,= x l0 t = 0, X23 Cofficient of Conelation: r= X2,4 FunctionaL Relationships : X2. EXAMPLE CALCULATON )"=.00457x03 b = x 02 a = X2.5 Calculated Vartances: D = x 0 " B = x l0 5 C (variance of b)= x 06 A (variance of a)= x l0 5 o n2(enor variance for) x = x l}s o.'lerror variance for) y * x 05 X2.6 Confidence LimitsFor N = 32 and , the estimated mean and confidence intervals are given in Table X2.2. Student's / of and prediction TABLE X2. Example Data for Example Calculation Time, h 9. to Stress, psi Log Time, h ' Log Stress, outu f Point Time, h Stress, psl Log Time, h Log Stress, f 't l0 ] s A that 3ns. ials like l 'lO J s meress rof rdo rof ress
11 .$Jp o 2ss206 TABLE X2.2 Confidence Limits  M Time, h Mean 6056 cotl LOWer Confidence nterval LOWET Prediction nterval 577'l s 'l T ol ST SUMMARY OF CHANGES Committee D20 has identified the location of selected chanses to this standard since the last issue (D \ that may impact the use of this standard. () RPMP and RTRP acronyms in 3..6 and 3.l.7were corrected. (2) Note 7 was added. (3) was revised. (4). was revised. (5) 2.3 was revised. ASTM lnternational takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every five years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM lnternational Headquafters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may aftend. lf you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, at the address shown below. This standard is copyrighted by ASTM lnternational, 00 Barr Harbor Drive, PO Box C700, West Conshohocken, PA , United States. lndividual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at (phone), (fax), or ( ); or through the ASTM website ( Scope* T, i. This spe< mosetting resin filament windin are a classifica mechanical pro test, and markir.2 The valur as standard. Thr information pur.3 The follo test method pc standard does n' if any, associate of this standart practices and dt tions prior to ut Norn lthe te specification applie and reinforced poi only reinforced the Norr 2This s outside diameter to Nore 3There NorB 4For thr natural polymers. 2. Referenced l 2. ASTM Stc D 6l B Practic 'This specificatior Plastics and is the di Plastic Piping System Current edition ap approved in 97. Lai 2 For referenced A contact ASTM Custor Standards volume infc the ASTM website. Copyright O ASTM nterni 328
Standard Test Method for Elastic Properties of Elastomeric Yarns (CRE Type Tensile Testing Machines) 1
Designation: D 2731 01 Standard Test Method for Elastic Properties of Elastomeric Yarns (CRE Type Tensile Testing Machines) 1 This standard is issued under the fixed designation D 2731; the number immediately
More informationCopyright ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA , United States.
LastD 4429 93 standard and is intended only to provide the user of an ASTM standard an indication of what changes have been made to the previous version. Because it may not be technically possible to adequately
More informationA New Test Setup for Testing Polyethylene Tubes under Constant and Cyclic Internal Pressures
A New Test Setup for Testing Polyethylene Tubes under Constant and Cyclic Internal Pressures S. Vahidi, E. Schruba, Y. Sun, M. McCarthy, and Y. G. Hsuan Drexel University, Philadelphia, PA, USA Abstract
More informationStandard Test Method for Vicat Softening Temperature of Plastics 1
Designation: D 1525 00 Standard Test Method for Vicat Softening Temperature of Plastics 1 This standard is issued under the fixed designation D 1525; the number immediately following the designation indicates
More informationmodulus of elasticity the slope of the elastic portion of the stressstrain curve. The ratio of stress to corresponding strain below the propor
Designation: 96 Standard Test Method for Tension Testing of Wire Ropes and Strand 1 This standard is issued under the fixed designation ; the number immediately following the designation indicates the
More informationStandard Test Method for Water Absorption of Rigid Cellular Plastics 1
Designation: D 2842 01 Standard Test Method for Water Absorption of Rigid Cellular Plastics 1 This standard is issued under the fixed designation D 2842; the number immediately following the designation
More informationThe Use of ILI In Dent Assessments
The Use of ILI In Dent Assessments Prepared for: 2014 CRUG Conference Date: 11 September 2014 Prepared by: Rhett Dotson, PE Contributions from Dr. Chris Alexander and Markus Ginten Contents Current Dent
More informationStandard Test Method for Chipping Resistance of Coatings 1
Designation: D 3170 03 Standard Test Method for Chipping Resistance of Coatings 1 This standard is issued under the fixed designation D 3170; the number immediately following the designation indicates
More informationPVP Copyright 2009 by ASME
Proceedings of PVP 009 009 ASME Pressure Vessel and Piping Division Conference July 630, 009, Prague, Czech Republic PVP0097746 UPDATE OF THE TABULATED «M AND Y» VALUES IN THE NEW REVISIONS OF FRENCH
More informationHYDROGEN STANDARDIZATION INTERIM REPORT For
STP/PT003 Designator: Meta Bold 24/26 Revision Note: Meta Black 14/16 HYDROGEN STANDARDIZATION INTERIM REPORT For Tanks, Piping, and Pipelines Date of Issuance: June 6, 2005 This report was prepared as
More informationStandard Test Methods for Water Vapor Content of Electrical Insulating Gases by Measurement of Dew Point 1
Designation: D 2029 97 (Reapproved 2003) Standard Test Methods for Water Vapor Content of Electrical Insulating Gases by Measurement of Dew Point 1 This standard is issued under the fixed designation D
More informationStandard Test Methods for Shear Adhesion of PressureSensitive Tapes 1
Designation: D 3654/D 3654M 02 Standard Test Methods for Shear Adhesion of PressureSensitive Tapes 1 This standard is issued under the fixed designation D 3654/D 3654M; the number immediately following
More informationStandard Test Method for Infiltration Rate of Soils in Field Using DoubleRing Infiltrometer 1
This document is not an ASTM standard and is intended only to provide the user of an ASTM standard an indication of what changes have been made to the previous version. Because it may not be technically
More informationVACUUM TESTING PRECAST CONCRETE MANHOLES
1 OF 5 testing is a quick, safe and practical way to validate manhole system integrity. Manhole sections can be tested at the precast concrete plant prior to delivery or on site prior to backfilling. Here
More informationStandard Pneumatic Test Procedure Requirements for Piping Systems
the pressure equipment safety authority Standard Pneumatic Test Procedure Requirements for Piping Systems AB522 Edition 2, Rev. 1 Issued 20161024 Table of Contents FOREWORD... 1 1.0 INTRODUCTION...
More informationBursting strength of paper. 1. Scope
T 403 om97 OFFICIAL STANDARD 1926 TENTATIVE STANDARD 1952 OFFICIAL STANDARD 1974 CORRECTED 1976 OFFICIAL TEST METHOD 1985 CORRECTED 1985 REVISED 1991 REVISED 1997 1997 TAPPI The information and data contained
More informationCONTROL VALVE TESTING
The optimal functioning of the Control valve not only exists of sufficient body & seat tightness, but more important, the total "performance" of the valve and its controls! For an accurate and reliable
More informationEVALUATION SUBJECT: SPUNSTRAND STANDARD AND INSULATED UNDERSLAB DUCTS
ICCES Report ESR1681 Reissued 12/2017 This report is subject to renewal 12/2018 EVALUATION SUBJECT: SPUNSTRAND STANDARD AND INSULATED UNDERSLAB DUCTS DIVISION: 23 00 00 HEATING, VENTILATING AND AIR CONDITIONING
More informationWAVE PRESSURE DISTRIBUTION ON PERMEABLE VERTICAL WALLS
Abstract WAVE PRESSURE DISTRIBUTION ON PERMEABLE VERTICAL WALLS Hendrik Bergmann, Hocine Oumeraci The pressure distribution at permeable vertical walls is investigated within a comprehensive largescale
More informationSPECIFICATION FOR REPEATED LOAD TRIAXIAL (RLT) TESTING FOR PAVEMENT MATERIALS
SPECIFICATION FOR REPEATED LOAD TRIAXIAL (RLT) TESTING FOR PAVEMENT MATERIALS 1. SCOPE This specification details the six (6) stage permanent strain Repeated Load Triaxial (RLT) test for unbound and modified
More informationOrganisation Internationale de Métrologie Légale
Organisation Internationale de Métrologie Légale OIML INTERNATIONAL RECOMMENDATION Pressure balances Manomètres à piston OIML R 110 Edition 1994 (E) CONTENTS Foreword... 3 1 Scope... 4 2 Terminology...
More informationJEDEC STANDARD. Temperature Cycling. JESD22A104C (Revision of JESD22A104B) JEDEC SOLID STATE TECHNOLOGY ASSOCIATION MAY 2005
JEDEC STANDARD Temperature Cycling JESD22A104C (Revision of JESD22A104B) MAY 2005 JEDEC SOLID STATE TECHNOLOGY ASSOCIATION NOTICE JEDEC standards and publications contain material that has been prepared,
More informationOTIF = Intergovernmental Organisation for International Carriage by Rail (Bern) ECE = United Nations Economic Commission for Europe (Geneva)
Recognized technical code (Anerkanntes Technisches Regelwerk, ATR) for the construction, equipment, test, approval, and marking as transportable pressure equipment of composite tubes with a seamless, load
More informationDesign and Safety Document for the Vacuum Windows of the NPDGamma Liquid Hydrogen Target at SNS
Design and Safety Document for the Vacuum Windows of the NPDGamma Liquid Hydrogen Target at SNS Prepared: Checked: Approved: H. Nann W. Fox M. Snow The NPDGamma experiment is going to run at BL13 at SNS
More informationSmart Water Application Technologies (SWAT) TM
Smart Water Application Technologies (SWAT) TM Equipment Functionality Test Protocol Version 2.3 June 2014 SWAT Committee 8280 Willow Oaks Corporate Drive Suite 400 Fairfax, VA 22031 www.irrigation.org
More informationLEAP CO 2 Laboratory CO 2 mixtures test facility
LEAP CO 2 Laboratory CO 2 mixtures test facility THE PROJECT AIM CO 2 flows made available by several capture techniques are contaminated with impurities and this affects the design and operations of the
More informationASME Boiler & Pressure Vessel Code Analysis of the 1497 MHz HighCurrent Cryomodule Helium Vessel
1.0 Introduction ASME Boiler & Pressure Vessel Code Analysis of the 1497 MHz HighCurrent Cryomodule Helium Vessel Katherine Wilson 28 May 2007 To minimize the hazards associated with vacuum and pressure
More informationISO INTERNATIONAL STANDARD. Fluid power systems Orings Part 2: Housing dimensions for general applications
INTERNATIONAL STANDARD ISO 36012 First edition 20080615 Fluid power systems Orings Part 2: Housing dimensions for general applications Transmissions hydrauliques et pneumatiques Joints toriques Partie
More informationAIAA Brush Seal Performance Evaluation. P. F. Crudgington Cross Manufacturing Co. Ltd. Devizes, ENGLAND
AIAA 983172 Brush Seal Performance Evaluation P. F. Crudgington Cross Manufacturing Co. Ltd. Devizes, ENGLAND BRUSH SEAL PERFORMANCE EVALUATION AIAA983172 P. F. Crudgington Cross Manufacturing Co. Ltd
More informationLevel MEASUREMENT 1/2016
Level MEASUREMENT 1/2016 AGENDA 2 A. Introduction B. Float method C. Displacer method D. Hydrostatic pressure method E. Capacitance method G. Ultrasonic method H. Radar method I. Laser method J. Level
More informationMSC Guidelines for the Submission of Stability Test (Deadweight Survey or Inclining Experiment) Results
S. E. HEMANN, CDR, Chief, Hull Division References a. 46 CFR 170, Subpart F Determination of Lightweight Displacement and Centers of Gravity b. NVIC 1791 Guidelines for Conducting Stability Tests c. ASTM
More informationApplication Note AN107
SPEC Sensor TM Characterization & Calibration Considerations Scope This document is provided to describe the considerations needed to characterize, calibrate, verify and validate the measurement performance
More informationTEST FOR STABILOMETER VALUE OF BITUMINOUS MIXTURES
Test Procedure for TEST FOR STABILOMETER VALUE OF BITUMINOUS MIXTURES TxDOT Designation: Tex208F Effective Date: February 2005 1. SCOPE 1.1 Use this test method to determine the Hveem stability value
More informationSTD3V1M4_1.7.1_AND_ /15/2015 page 1 of 6. TNI Standard. ELV1M4 Sections and September 2015
page 1 of 6 TNI Standard ELV1M4 Sections 1.7.1 and 1.7.2 September 2015 Description This TNI Standard has been taken through all of the voting stages and has received consensus approval by the TNI membership.
More informationDetermination of the Design Load for Structural Safety Assessment against Gas Explosion in Offshore Topside
Determination of the Design Load for Structural Safety Assessment against Gas Explosion in Offshore Topside Migyeong Kim a, Gyusung Kim a, *, Jongjin Jung a and Wooseung Sim a a Advanced Technology Institute,
More informationApplying Hooke s Law to Multiple Bungee Cords. Introduction
Applying Hooke s Law to Multiple Bungee Cords Introduction Hooke s Law declares that the force exerted on a spring is proportional to the amount of stretch or compression on the spring, is always directed
More informationStandard Specification for Anesthetic Gas Scavenging Systems Transfer and Receiving Systems 1
Designation: F 1343 02 Standard Specification for Anesthetic Gas Scavenging Systems Transfer and Receiving Systems 1 This standard is issued under the fixed designation F 1343; the number immediately following
More informationSept 23, 2014 LAB MANUAL
Sept 23, 2014 LAB MANUAL 1000.0 1000 STANDARD PRACTICES 1000.1 CALCULATIONS and FORMS Throughout this manual there are test calculation procedures. These calculations are provided so that a technician
More information5.1 Introduction. Learning Objectives
Learning Objectives 5.1 Introduction Statistical Process Control (SPC): SPC is a powerful collection of problemsolving tools useful in achieving process stability and improving capability through the
More informationCommonwealth of Pennsylvania PA Test Method No. 742 Department of Transportation October Pages LABORATORY TESTING SECTION. Method of Test for
Commonwealth of Pennsylvania PA Test Method No. 742 Department of Transportation 14 Pages LABORATORY TESTING SECTION Method of Test for BITUMEN CONTENT OF BITUMINOUS CONCRETE MIXTURES (Pennsylvania Pycnometer
More informationRetention Time Locking: Concepts and Applications. Application
Retention Time Locking: Concepts and Applications Application Gas Chromatography December 1997 Authors Vince Giarrocco Bruce Quimby Matthew Klee Agilent Technologies, Inc. 2850 Centerville Road Wilmington,
More informationSECTION BUTTERFLY VALVES
SECTION 15112 BUTTERFLY VALVES PART 1 GENERAL 1.01 SUMMARY A. All butterfly valves shall be of the tight closing, rubber seated type and fully comply with the latest revision of AWWA Standard C504, Class
More informationSECTION 25 TESTING AND DISINFECTING WATER MAINS General
SECTION 25 TESTING AND DISINFECTING WATER MAINS 251.01 Scope 251 General This section describes the requirements for pressure and leak testing, and disinfecting of water mains and appurtenances, including
More informationAPPLYING VARIABLE SPEED PRESSURE LIMITING CONTROL DRIVER FIRE PUMPS. SEC Project No
APPLYING VARIABLE SPEED PRESSURE LIMITING CONTROL DRIVER FIRE PUMPS SEC Project No. 1803007000 November 20, 2006 TABLE OF CONTENTS I. ABSTRACT...1 II. INTRODUCTION...1 III. HISTORY...2 IV. VARIABLE SPEED
More informationSIZING AND CAPACITIES OF GAS PIPING
SIZING AND CAPACITIES OF GAS PIPING A.1 General piping considerations. The first goal of determining the pipe sizing for a fuel gas piping system is to make sure that there is sufficient gas pressure at
More informationBoyle s Law: PressureVolume Relationship in Gases. PRELAB QUESTIONS (Answer on your own notebook paper)
Boyle s Law: PressureVolume Relationship in Gases Experiment 18 GRADE LEVEL INDICATORS Construct, interpret and apply physical and conceptual models that represent or explain systems, objects, events
More informationINTERNATIONAL HYDROGRAPHIC SURVEY STANDARDS
INTERNATIONAL HYDROGRAPHIC SURVEY STANDARDS by Gerald B. MILLS 1 I. Background The International Hydrographic Organization (IHO) traces its origin to the establishment of the International Hydrographic
More informationPaint Brush Handle. Julia Carlson Heather Curtin Julia Hamlin. Western Washington University. March 12, 2003
Paint Brush Handle Julia Carlson Heather Curtin Julia Hamlin Western Washington University March 12, 2003 Society of Plastics Engineers Blow Molding Division 2003 Student Design Competition Recycled Paintbrush
More informationNATURAL GAS MAINTENANCE. Part 192 Subpart "M"
NATURAL GAS MAINTENANCE Part 192 Subpart "M" CONTACT INFORMATION Pamela West Pipeline Safety Specialist U.S. Department of Transportation PHMSA Inspector Training and Qualifications Main: (405) 6862310
More informationISO INTERNATIONAL STANDARD
INTERNATIONAL STANDARD ISO 907316 First edition 20071201 Textiles Test methods for nonwovens Part 16: Determination of resistance to penetration by water (hydrostatic pressure) Textiles Méthodes d'essai
More informationBODY OF KNOWLEDGE API510 PRESSURE VESSEL INSPECTOR CERTIFICATION EXAMINATION
BODY OF KNOWLEDGE API510 PRESSURE VESSEL INSPECTOR CERTIFICATION EXAMINATION May and September, 2017 and January 2018 (Replaces May 2016) API Authorized Pressure Vessel Inspectors must have a broad knowledge
More informationISO/TC 131/SC Hydraulic fluid power Test methods for hoses and hose assemblies
DRAFT INTERNATIONAL STANDARD ISO/DIS 6605 ISO/TC 131/SC 4 Secretariat: ANSI Voting begins on: Voting terminates on: 20160203 20160503 Hydraulic fluid power Test methods for hoses and hose assemblies
More informationWSC Performance Standard and Recommended Installation Procedures for Sanitary Water Well. Pitless Adapters, Pitless Units, And Well Caps
WSC Performance Standard and Recommended Installation Procedures for Sanitary Water Well Pitless Adapters, Pitless Units, And Well Caps History of the WSC PAS Standard he Water Systems Council (WSC) has
More informationTECHNICAL DATA OBSOLETE
June 1, 2008 Foam 240a 1. DESCRIPTION The Chemguard Bladder Tank is one component in a balanced pressure foam proportioning system. It requires no external power, other than the water pressure to ensure
More informationGases and Pressure SECTION 11.1
SECTION 11.1 Gases and In the chapter States of Matter, you read about the kineticmolecular theory of matter. You were also introduced to how this theory explains some of the properties of ideal gases.
More informationAir Pycnometer. Operating Manual. UmweltGeräteTechnik GmbH
Operating Manual Air Pycnometer Version: 24/05/17 UmweltGeräteTechnik GmbH Eberswalder Str. 58 D15374 Müncheberg phone: +49 (0) 33 43 289 575 fax: +49 (0) 33 43 289 573 email: info@ugtonline.de
More informationLOW PRESSURE EFFUSION OF GASES adapted by Luke Hanley and Mike Trenary
ADH 1/7/014 LOW PRESSURE EFFUSION OF GASES adapted by Luke Hanley and Mike Trenary This experiment will introduce you to the kinetic properties of lowpressure gases. You will make observations on the
More informationThe Discussion of this exercise covers the following points:
Exercise 32 Orifice Plates EXERCISE OBJECTIVE In this exercise, you will study how differential pressure flowmeters operate. You will describe the relationship between the flow rate and the pressure drop
More informationDuPont Kalrez. Oil and Gas Product Selector Guide. Technical Information April 2017
DuPont Kalrez Oil and Gas Product Selector Guide Technical Information April 2017 DuPont has more than 30 years of experience providing perfluoroelastomer seals to the oil and gas industry. Over this time,
More informationCONTROL VALVE WHAT YOU NEED TO LEARN?
CONTROL VALVE WHAT YOU NEED TO LEARN? i) The control valve characteristics refers to the relationship between the volumetric flowrate F (Yaxis) through the valve AND the valve travel or opening position
More informationStandard Test Method for Air Content of Freshly Mixed Concrete by the Pressure Method 1
Designation: C 231 03 Standard Test Method for Air Content of Freshly Mixed Concrete by the Pressure Method 1 This standard is issued under the fixed designation C 231; the number immediately following
More informationAPPENDIX A RECOMMENDED RULES FOR SIZING THE WATER SUPPLY SYSTEM CHART A 1.2 FRICTION LOSSES FOR DISKTYPE WATER METERS 11/2"
RECOMMENDED RULES FOR SIZING THE WATER SUPPLY SYSTEM Because of the variable conditions encountered, it is impractical to lay down definite detailed rules of procedure for determining the sizes of water
More informationLiquid level measurement using hydrostatic pressure and buoyancy
iquid level measurement using hydrostatic pressure and buoyancy This worksheet and all related files are licensed under the Creative Commons Attribution icense, version 1.0. To view a copy of this license,
More informationDEVELOPMENT OF A ROBUST PUSHIN PRESSUREMETER
DEVELOPMENT OF A ROBUST PUSHIN PRESSUREMETER Roger Failmezger, P.E. InSitu Soil Testing, L.C., Lancaster, Virginia, USA ABSTRACT A pushin pressuremeter was developed using slotted steel casing with
More informationCHEMICAL. Straight cut rod is provided in the materials listed below and includes nuts / washers.
161 STRAIGHT CUT ROD Straight cut rod is provided in the materials listed below and includes nuts / washers. Straight Rod 221/2 Bent Rod A 307 THREADED ANCHOR ROD, ZINC PLATED (ASTM B633, CLEAR CHROMATE)
More informationLOW PRESSURE EFFUSION OF GASES revised by Igor Bolotin 03/05/12
LOW PRESSURE EFFUSION OF GASES revised by Igor Bolotin 03/05/ This experiment will introduce you to the kinetic properties of lowpressure gases. You will make observations on the rates with which selected
More informationServing. Petrochemicals Power Semiconductor Waste Treatment Oil & Gas Transmission Lines Bulk Gas Plants
Serving Petrochemicals Power Semiconductor Waste Treatment Oil & Gas Transmission Lines ulk Gas Plants Mining & Metals Pharmaceuticals Pulp & Paper Mills Sugar Mills Nuclear Desalinization Plants NOTES:
More informationFATIGUE, FAILSAFE, AND DAMAGE TOLERANCE EVALUATION OF METALLIC STRUCTURE FOR NORMAL, UTILITY, ACROBATIC, AND COMMUTER CATEGORY AIRPLANES
AC 2313A FATIGUE, FAILSAFE, AND DAMAGE TOLERANCE EVALUATION OF METALLIC STRUCTURE FOR NORMAL, UTILITY, ACROBATIC, AND COMMUTER CATEGORY AIRPLANES September 29, 2005 For sale by the Superintendent of
More informationStandard Recommended Practice. Field Measurement of Surface Profile of Abrasive BlastCleaned Steel Surfaces Using a Replica Tape
NACE Standard RP02872002 Item No. 21035 Standard Recommended Practice Field Measurement of Surface Profile of Abrasive BlastCleaned Steel Surfaces Using a Replica Tape This NACE International standard
More informationMSC Guidelines for Independent Fuel Tanks
References: Contact Information a. 46 CFR 58.50 (Independent Fuel Tanks) b. 46 CFR 119.440 (Independent Fuel Tanks) c. 46 CFR 182.440 (Independent Fuel Tanks) C. J. Robuck, LCDR, Chief, Engineering Division
More informationGAS SUPPLY DESIGN GUIDE
GAS SUPPLY DESIGN GUIDE Natural Gas, Propane Gas, or Dual Fuel Fired Modulating, Condensing Boilers BENCHMARK Series GasFired Boilers For models: BMK750 to BMK6000 Last Update: 06/20/2014 PR1 06/20/14
More informationCertification of AMS acc. EN 15267, Part 3  Overview and First Experience 
Certification of AMS acc. EN 15267, Part 3  Overview and First Experience  Dr. Wolfgang Jockel, Martin Schneider, TÜV Rheinland Group, D51105 Cologne / Germany 1. Introduction A new basis for the certification
More informationSUPPORTING NOTES FOR THE EVALUATION OF UNBOUND ROAD BASE AND SUBBASE AGGREGATES
SUPPORTING NOTES FOR THE EVALUATION OF UNBOUND ROAD BASE AND SUBBASE AGGREGATES (These notes are guidelines only and must not be included in the Contract Documents). 1. SCOPE These Notes are guidelines
More informationPerformance Verification of BioTek s Precision 2000 using Artel s Multichannel Volume Verification (MVV ) System
Performance Verification of BioTek s Precision 2000 using Artel s Multichannel Volume Verification (MVV ) System Authors: Paul Held 1, John Bradshaw 2, Jason Greene 1, Alex Rogers 2, and Tanya Knaide 2
More informationDNVGLCP0187 Edition March 2016
CLASS PROGRAMME Type approval DNVGLCP0187 Edition March 2016 The electronic pdf version of this document, available free of charge from http://www.dnvgl.com, is the officially binding version. FOREWORD
More informationFinite Element Analysis of an Aluminium Bike Frame
Finite Element Analysis of an Aluminium Bike Frame Word Count: 1484 1 1. Introduction Each new bike model must pass a series of structural tests before being released for public retail. The purpose of
More informationREPORT HOLDER: FRAMECAD LICENSING LTD. POST OFFICE BOX 1292 AUCKLAND 1140 NEW ZEALAND EVALUATION SUBJECT: COLD FORMED STEEL C SHAPES AND TRACKS
0 Most Widely Accepted and Trusted ICC ES Evaluation Report ICC ES 000 (800) 423 6587 (562) 699 0543 www.icc es.org ESR 2361 Reissued 05/2017 This report is subject to renewal 05/2019. DIVISION: 05 00
More informationHigh Speed Rail Tunnel Aerodynamics: Transient pressure and loadings on fixed tunnel equipment
High Speed Rail Tunnel Aerodynamics: Transient pressure and loadings on fixed tunnel equipment Mohammad Tabarra & Richard Sturt Arup, UK Summary: Trains entering tunnels at high speeds can generate highly
More informationTESTING OF BELIMO PRESSURE INDEPENDENT CHARACTERIZED CONTROL VALVES
TESTING OF BELIMO PRESSURE INDEPENDENT CHARACTERIZED CONTROL VALVES November, 25 Submitted by: Iowa Energy Center Address: DMACC, 26 S. Ankeny Blvd. Ankeny, IA 521 Phone: 515.965.755 Fax: 515.965.756 Web
More informationGolf Ball Impact: Material Characterization and Transient Simulation
12 th International LSDYNA Users Conference Blast/Impact(1) Golf Ball Impact: Material Characterization and Transient Simulation Xiaohu Liu, David Quinn and Jorgen Bergström Veryst Engineering, LLC 47A
More informationMTS Restan. Automatic System for Residual Stress Measurement by HoleDrilling
Automatic System for Residual Stress The MTS3000  Restan system for measuring residual stresses Fully automatic drilling and acquisition process ensuring high repeatability High speed drilling (400,000
More informationFlange Bolt Torquing. for Resistoflex PlasticLined Piping Products. Torquing. Retorquing. Hydrotesting. Annual retorquing
Flange Bolt Torquing for Resistoflex PlasticLined Piping Products Torquing When assembling flange connections, always use a full complement of clean, new high strength A193B7 bolting. If using stainless
More informationFatigue Test Results and Analysis 42 Piston Provost Wings
t" O'3 R. & M. No. 3474 Z MINISTRY OF TECHNOLOGY AERONAUTICAL RESEARCH COUNCIL Fatigue Test Results and Analysis 42 Piston Provost Wings of by H. E. PARISH, A.F.R.Ae.S. LONDON: HER MAJESTY'S STATIONERY
More informationTG119 IMRT Commissioning Tests Instructions for Planning, Measurement, and Analysis Version 10/21/2009
TG119 IMRT Commissioning Tests Instructions for Planning, Measurement, and Analysis Version 10/21/2009 DISCLAIMER: This publication and associated spreadsheets and digital files are based on sources and
More informationInternational Journal of Technical Research and Applications eissn: , Volume 4, Issue 3 (MayJune, 2016), PP.
DESIGN AND ANALYSIS OF FEED CHECK VALVE AS CONTROL VALVE USING CFD SOFTWARE R.Nikhil M.Tech Student Industrial & Production Engineering National Institute of Engineering Mysuru, Karnataka, India 570008
More informationBoyle s Law: PressureVolume Relationship in Gases
Boyle s Law: PressureVolume Relationship in Gases The primary objective of this experiment is to determine the relationship between the pressure and volume of a confined gas. The gas we will use is air,
More informationNotice for Pressure Special Equipment Manufacture Licensing
AQSIQ Notice No.151 (2012) Notice for Pressure Special Equipment Manufacture Licensing To further enhance the implementation of the manufacture licensing system to imported pressure special equipment,
More informationAPI510 PRESSURE VESSEL INSPECTOR
BODY OF KNOWLEDGE API510 PRESSURE VESSEL INSPECTOR CERTIFICATION EXAMINATION July 2013 (Replaces July 2012) API Authorized Pressure Vessel Inspectors must have a broad knowledge base relating to maintenance,
More informationVessels subject to External Pressure
Basic principles of compressive force Vessels subject to External Pressure Before After The result of just air pressure! Presented by: Ray Delaforce Basic principles of compressive force Consider For a
More informationAPPENDIX A RECOMMENDED RULES FOR SIZING THE WATER SUPPLY SYSTEMS CHART A1 FRICTION LOSSES FOR DISKTYPE WATER METERS 11/2"
RECOMMENDED RULES FOR SIZING THE WATER SUPPLY SYSTEMS Because of the variable conditions encountered, it is impractical to lay down definite detailed rules of procedure for determining the sizes of water
More informationCasing Design. Casing Design. By Dr. Khaled Elshreef
Casing Design By Dr. Khaled Elshreef 1 Casing Design CONTENTS Function of Casing Casing Types & Tools Strength Properties Casing Specification Casing Design 2 1 RUNNING AND CEMENTING CASING Reasons for
More informationHYDROSTATIC LEAK TEST PROCEDURE
This information is proprietary and shall not be disclosed outside your organization, nor shall it be duplicated, used or disclosed for purposes other than as permitted under the agreement with Kinetics
More informationTESTING APPLICATION STANDARD (TAS)
TESTING APPLICATION STANDARD (TAS) No. 00(A)9 TEST PROCEDURE FOR WIND AND WIND DRIVEN RAIN RESISTANCE AND/OR INCREASED WINDSPEED RESISTANCE OF SOFFIT VENTILATION STRIP AND CONTINUOUS OR INTERMITTENT VENTILATION
More informationEffect of Coiled Capillary Tube Pitch on Vapour Compression Refrigeration System Performance
Effect of Coiled Capillary Tube Pitch on Vapour Compression Refrigeration System Performance Mutalubi Aremu Akintunde Federal University of Technology, Department of Mechanical Engineering Akure, Ondo
More informationFigure 1 Schematic of opposing air bearing concept
Theoretical Analysis of Opposing Air Bearing Concept This concept utilizes air bearings to constrain five degrees of freedom of the optic as shown in the figure below. Three pairs of inherently compensated
More informationChapter Pipette service & maintenance. Pipette specifications according to ISO Repair in the lab or return for service?
Pipette specifications according to ISO 8655 Chapter 5 5.1 The ISO 8655 standard gives the accuracy and precision limits as both absolute and relative values. Specifications will depend on the technique
More informationA hose layline contains important information for specifying the replacement assembly: manufacturer, hose trade name, working pressure and hose ID.
CONTENTS Introduction Pressure Pressure Drop Temperature Rating Bend Radius Conclusion Additional Information SIDEBAR: Understanding Hydraulic Hose Reinforcement INTRODUCTION Hydraulic hose has a finite
More informationASSESSMENT AND ANALYSIS OF PIPELINE BUCKLES
ASSESSMENT AND ANALYSIS OF PIPELINE BUCKLES GE Oil & Gas PII Pipeline Solutions Inessa Yablonskikh Principal Consultant Aberdeen, November, 14 th 2007 Assessment And Analysis Of Pipeline Buckles Introduction
More informationCOMPRESSION TUBE FITTINGS
COMPRESSION TUBE FITTINGS 1/16 THROUGH 2 2 MM THROUGH 50 MM LETLOK TUBE FITTINGS DESCRIPTION The HAMLET GROUP has produced high quality tube and pipe fittings in various materials for high pressure applications
More informationEquation 1: F spring = kx. Where F is the force of the spring, k is the spring constant and x is the displacement of the spring. Equation 2: F = mg
1 Introduction Relationship between Spring Constant and Length of Bungee Cord In this experiment, we aimed to model the behavior of the bungee cord that will be used in the Bungee Challenge. Specifically,
More information